### arXiv:cond-mat/9606030v1 5 Jun 1996

### Hall Resistivity in Ferromagnetic Manganese-Oxide Compounds

Liang-Jian Zou

*CCAST (World Laboratory) P.O.Box 8730, Beijing, 100080*

*Institute of Solid State Physics, Academia Sinica, P.O.Box 1129, Hefei 230031, China*∗

Abstract

Temperature-dependence and magnetic field-dependence of the Hall effect and the magnetic property in manganese-oxide thin films are studied. The spontaneous magnetization and the Hall resistivity are obtained for a various of magnetic fields over all the temperature. It is shown that the Hall resistivity in small magnetic field is to exhibit maximum near the Curie point, and strong magnetic field moves the position of the Hall resistivity peak to much high temperature and suppresses the peak value. The change of the Hall resistance in strong magnetic field may be larger than that of the diagonal ones. The abnormal Hall resistivity in the ferromagnetic manganese-oxide thin-films is attributed to the spin-correlation fluctuation scattering.

*PACS No.: 73.50.Jt, 73.50.Bk*

I. INTRODUCTION

Recently colossal negative magnetoresistance (MR) effect has been found in ferromagnetic perovskite-like La1−xRxMnO3 and Nd1−xRxMnO3 ( R =Ba, Sr, Ca, Pb, etc. ) [ 1 - 4 ] thin

films. In epitaxial La1−xCaxMnO3 and Nd1−xSrxMnO3 thin films, the resistivity in applied

magnetic field decreases several order in magnitude under strong magnetic field, which is much larger than that found in ferromagnetic/nonmagnetic metallic multilayers. Since such a huge MR change has potential application for magnetic sensor, magnetic recording and many other aspects, it also presents another possible MR mechanism which is different from that in magnetic multilayer, it arises extensive attention and interests in the past two years [ 5 - 12 ].

Undoped LaMnO3 is an antiferromagnetic insulator [ 13 - 16 ], its magnetic structure and

magnetic properties had been studied in the early of 1950’s. After the substitution of a part
of trivalent La or Nd ions by Ca, Sr, Pb, Ba or other divalent elements, Mn+3 _{and Mn}+4

ions coexist, the valence fluctuation between them is thus assumed to be important and may contribute to the hopping conductivity and other transport properties. In the substitution of La or Nd ions, La1−xRxMnO3 and Nd1−xRxMnO3 systems may occur the metal-insulator

transition, the electronic states in doped systems at the edge of metal-insulator transition can be heavily affected by the long-range magnetic order and the external magnetic field. Some mechanism have been proposed to explain the colossal MR effect in these systems [ 8 - 11 ]. The magnetic polaron mechanism [ 1 - 3 ], the spin disorder scattering [ 8, 9 ] and the metal-insulator transition [ 11 ] induced by the magnetic field seem to be difficult to explain the colossal MR behavior in strong magnetic field over all the temperature satisfactorily.

In recent study [ 12 ], another possible mechanism for these ferromagnetic La1−xRxMnO3

and Nd1−xRxMnO3 thin films is proposed to explain the colossal MR. It is suggested that the

abnormal large MR in these compounds is induced by the spin-spin correlation fluctuation scattering, the magnetic property and the diagonal resistivity in different magnetic fields agree with the experimental results very well. The Hall effect is one of the important properties and may distinguish the present mechanism from the metal-insulator transition mechanism [11], so it is useful to predict the Hall resistivity behavior. In this letter, the Hall resistivity and the magnetic property for temperature T and magnetic field B are obtained. The rest is arranged as following, in Sec.II, the formalism is described; the results and discussions are given in Sec.III, and the conclusion is drawn in Sec.IV.

II. FORMALISM

In La1−xRxMnO3 and Nd1−xRxMnO3 compounds, because of the crystalline field effect,

the 3d energy level of the Mn ion is split into the low-energy triplet, t2g, and the high-energy

doublet, eg, therefore the three d-electrons of Mn+3 and Mn+4 ions first fill the low t2g band,

and the extra d-electrons in Mn+3 _{will have to fill the high e}

g band, these two bands are

separated about 1.5 eV [ 17 ]. Thus the three d-electrons in filled t2g band forms a localized

core spin through the strong Hund’s coupling [ 13 - 16 ], the core spins tend to align parallelly
through the double exchange interaction through Mn+3_{-O}−2_{-Mn}+4 _{and form ferromagnetic}

background. The electrons in eg band are mobile and responsible for electric conduction in

these systems. In this framework, the model Hamiltonian for the mobile electrons moving in the ferromagnetic background is described:

H0 =
X
kσ
(ǫk− σµBB)c†kσckσ−
X
<ij>
*AS*i· Sj −
X
i
gµBBSiz (2)
V = −J
N
X
ikq
X
µν
eiqRi
Si· c†k+qµσµνckν (3)

Where H0 describes the bare energies of the mobile d-electrons and the ferromagnetic

back-ground, V is the coupling between the mobile electrons and the core spins. In Eq.(2), ǫk represents the energy spectrum of mobile (or conduction) electrons with respect to the

Fermi energy EF*; A denotes the effective ferromagnetic exchange constant between *

man-ganese ions, and only the nearest-neighbor interaction is considered; -gµBB is Zeemann

energy in the magnetic field B. In Eq.(3), the conduction electron is scattered from state kν to state k+qµ by the localized spin Si; J denotes the coupling between the conduction

electrons and the core spins. One notes that in the external magnetic field and the internal molecular field of ferromagnetically ordered state, the conduction band of the system will be split, this splitting is to move the position of the conduction band with respect to the Fermi surface, thus the mean-field spectrum of the conduction electron with state kσ is ǫkσ = ǫk− σ(µBB + J < Sz >).

By the scattering theory [12], the lifetime of the conduction electrons between two
scat-terings, τ , is :
τ−1 = π
h
J2_{D(0)}
4
X
kqσ
fkσ(1 − fkσ)fk+q¯σ(1 − fk+q¯σ)[< Sq−S−q+ > + (4)
< Sq+S
−
−q > +8 < S
z
qS
z
−q >]

Where D(0) is the density of states of the conduction electrons near the Fermi surface, Dirac-Fermi distribution function fk = 1/[eβ(ǫk−ǫF)+ 1]. Then one can obtain the diagonal

concentration, and m the effective mass. With the diagonal resistivity, one can easily derive the Hall conductivity: in steady-state,

σH =

σ2 xx

neBef f (5)

or the Hall resistivity:

ρH =

ne Bef f

ρ2_{xx} (5′_{)}

where Bef f is effective field, Bef f= |B + zA < S > /µB|.

From to Eqs.(4) and (5), one could qualitatively understand the temperature-dependence of the Hall resistivity. At zero-temperature limit (T → 0 K), ρxx approaches zero because

of the Pauli exclusion principle, so ρH(T → 0) ≈ 0; however at high temperature limit

(T >> Tc, EF), ρxx in different magnetic field approaches the same value, the Hall

resistiv-ity mainly depends on the effective magnetic field. In this situation, the diagonal and the Hall resistivities may exhibit some different behaviors. In the mediated temperature range (0<kBT << EF), especially at the temperature near the Curie point, the diagonal resistivity

exhibits a maximum, therefore the Hall resistivity is also to exhibit a maximum, however, because of the effect of magnetic field, the position of the maximum of the Hall resistivity is smaller than that of the diagonal ones.

III. RESULTS AND DISCUSSIONS

In quasi-2-dimensional systems, the lattice constant is a=3.89 ˚A, and the coordinate number is z=4. The theoretical parameters is from La-Ca-Mn-O system, while the results can be applied for other similar systems. In the calculation, several parameters need to be determined by the experiments and the electronic structure calculation, for simplicity, the

reduced resistivity is adopted here.

The dependence of the spontaneous magnetization and the Hall resistivity on tempera-ture is shown in Fig.1, for comparison, the diagonal resistivity is also shown in Fig.1. The ferromagnetic-paramagnetic transition occurs within a wide temperature range, because of the critical fluctuation and the low-dimensional character, the temperature relation of the spontaneous magnetization has a long tail, the transition temperature is broaded signifi-cantly. The electrons moving in the transverse direction is also scattered by the spin-spin correlation fluctuation near the critical point, therefore the Hall resistivity also exhibits a maximum. In the meantime, the magnetic field B affects the cyclotron movement of the conduction electrons, the Hall resistivity decreases with B, so the maximum of the Hall re-sistivity will not appear at the same position as that of the diagonal rere-sistivity, the position of the maximum moves to low temperature. It can be seen clearly in Fig.1.

The field-dependence of the Hall resistivity at different temperature is shown in Fig.2. One notes that the Hall resistivity decreases monotonously when the external magnetic field is increased. The descent resistivity with the increase of magnetic field is due to the suppress of the spin-spin correlation fluctuation scattering. Below Tc, the spin-spin correlation is

long range, the applied magnetic field has strong effect on the scattering, so the change of the Hall resistivity is large (See the Curves (1) and (2)); while above Tc, the

short-range spin-spin correlation fluctuation dominates the scattering of conduction electrons, the external magnetic field has weak effect, so the Hall resistivity exhibits weak dependence on the magnetic field.

mag-netic field and by the spin-correlation scattering, the change of the Hall resistivity may be larger than the diagonal resistivity with the variation of the magnetic field. In the present mechanism, from the curve (1) in Fig.2, the Hall resistivity may decrease two to three orders in magnitude, for comparison, the diagonal resistivity only changes one to two orders in magnitude.

IV. CONCLUSION

In conclusion, we have studied the Hall resistivity and the magnetic property of the ferro-magnetic manganese-oxide compounds. The temperature-dependence of the Hall resistivity is to exhibit a maximum below the peak position of the diagonal resistivity, and the change of Hall resistivity in magnetic field will be larger than that of diagonal resistivity. The spin-spin correlation scattering between the conduction electrons and the localized spin-spins is the intrinsic mechanism of the abnormal Hall resistivity in La-R-Mn-O and Nd-R-Mn-O com-pounds near the transition point. Further experiments is desired to verify our predictions.

Acknowledgement: This work is financially supported by the Grant of National Natural Science Funds of China No.19577101.

REFERENCES * mailing address

*1. R. M. Kusters, J. Singleton, D. A. Keen, R. McGreevy and W. Hayes, Physica B155*
362 (1989).

*2. R. Von Helmolt, J. Wecker, B. Holzapfeil, L. Schultz and K. Samwer Phys. Rev. Lett.*
71 *2331 (1993). R. Von Helmolt, J. Wecker, and K. Samwer J. Appl. Phys. 76, 6925*
(1994).

3. S. Jin, T. H. Tiefel, M. McCormack, R. A. Fastnacht, R. Ramesh, and L, H, Chen

*Science. 264 413 (1994). J. Appl. Phys. 76, 6929 (1994).*

*4. S. Jin, H. M. O’Bryan, T. H. Tiefel, M. McCormack, and W. W. Rhodos Appl. Phys.*

*Lett 66, 382 (1995).*

5. G. C. Xiong, Q. Li, H. L. Ju, S. N. Mao, L. Senpati, X. X. Xi, R. L. Greene, and T.
*Venkatesan, Appl. Phys. Lett 66, 1427 (1995).*

*6. H. L. Ju, C. Kwon, Qi Li, L.Greene and T. Vankateson, Appl. Phys. lett. 65, 2106*
(1994).

*7. P. Schiffer, A. P. Ramirez, W. Bao and S-W. Cheong, Phys. Rev.Lett. 75, 3336 (1995).*
*8. N. Furukawa, J. Phys. Soc Jpn, 63, 3214 (1994).*

*9. J. Inoue and S. Maekawa, Phys. Rev. Lett 74, 3407 (1995).*

*11. A. Urushibara, Y. Moritomo, T. Arima, A. Asamitsu, G. Kido and Y. Tokuya, Phys.*

*Rev. B 51, 14103 (1995). Y. Moritomo, A. Asamitsu, and Y. Tokuya, Phys. Rev. B*

51, 16491 (1995).

*12. Liang-Jian Zou, X. G. Gong, Q. Q. Zheng and C Y. Pan, J. Appl. Phys., 78, No.4*
*(1996); Phys. Rev. B, submitted.*

*13. C. Zener, Phys. Rev., 81, 440 (1951); 82, 403 (1951).*

*14. E. O. Wollen and W. C. Koehler, Phys. Rev., 100, 545 (1955)*
*15. J. B. Goodenough, Phys. Rev., 100, 564 (1955)*

*16. P. G. De Gennes, Phys. Rev., 118, 141 (1960)*

Figures Captions

Fig. 1. Temperature-dependence of the spontaneous magnetization, the Hall resistivity and
*the diagonal resistivity in magnetic field. Theoretical parameters for calculation: A=145.5*
*K, J=350 K. B=15 T (1) spontaneous magnetization, (2) Hall resistivity, and (3) diagonal*
resistivity.

Fig. 2. Dependence of the Hall resistivity on the magnetic field at different temperature.
*Theoretical parameters: A=145.5 K, J=350 K, (1) T=50 K, (2) T=100 K, (3) T=80 K.*